The formation of peroxide degradation products of photochromic triphenylimidazolyl radical-dimers.
Edkins, Robert M.; Probert, Michael R.; Fucke, Katharina; Robertson, Craig M.; Howard, Judith A. K.; Beeby, Andrew; Physical chemistry chemical physics : PCCP 15 (2013) 7848–7853; doi:10.1039/c3cp50757b

data_7211295
_publ_section_title
;
 The formation of peroxide degradation products of photochromic
 triphenylimidazolyl radical-dimers.
;
_journal_issue                   20
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              7848
_journal_page_last               7853
_journal_paper_doi               10.1039/c3cp50757b
_journal_volume                  15
_journal_year                    2013
_chemical_formula_moiety         'C50 H46 N4 O2'
_chemical_formula_sum            'C50 H46 N4 O2'
_chemical_formula_weight         734.91
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2012-03-27
_audit_creation_method
;
Olex2 1.1
(compiled Nov 1 2011 20:42:30, GUI svn.r3906)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 93.7920(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   16.0313(4)
_cell_length_b                   30.9627(9)
_cell_length_c                   16.5171(5)
_cell_measurement_reflns_used    9740
_cell_measurement_temperature    100
_cell_measurement_theta_max      63.120
_cell_measurement_theta_min      3.038
_cell_volume                     8180.7(4)
_computing_cell_refinement       'SAINT v7.68A (Bruker, 2009)'
_computing_data_collection       'Proteum2 (Bruker, 2010)'
_computing_data_reduction        'SAINT v7.68A (Bruker, 2009)'
_computing_molecular_graphics
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_publication_material
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_structure_refinement
;
olex2.refine (L.J. Bourhis, O.V. Dolomanov, R.J. Gildea, J.A.K. Howard,
H. Puschmann, in preparation, 2011)
;
_computing_structure_solution
;
XS, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_diffrn_ambient_temperature      100
_diffrn_detector                 'CCD area detector'
_diffrn_detector_type            'Bruker Pt 135 CCD area detector'
_diffrn_measured_fraction_theta_full 0.962
_diffrn_measured_fraction_theta_max 0.962
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'Bruker Pt 135 CCD area detector'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_collimation    'focused optics'
_diffrn_radiation_monochromator  'Bruker Helios multilayer optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54188
_diffrn_radiation_xray_symbol    K-L~3~
_diffrn_reflns_av_R_equivalents  0.0480
_diffrn_reflns_av_unetI/netI     0.0338
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       35
_diffrn_reflns_limit_k_min       -35
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            62341
_diffrn_reflns_theta_full        63.30
_diffrn_reflns_theta_max         63.30
_diffrn_reflns_theta_min         2.76
_diffrn_source                   'Microstar rotating anode'
_diffrn_source_target            Cu
_diffrn_source_type              'rotating anode'
_exptl_absorpt_coefficient_mu    0.570
_exptl_absorpt_correction_T_max  0.7523
_exptl_absorpt_correction_T_min  0.6656
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2008/1 (Bruker,2008) was used for absorption correction.
R(int) was 0.0947 before and 0.0719 after correction.
The Ratio of minimum to maximum transmission is 0.8848.
The \l/2 correction factor is 0.0015.
;
_exptl_crystal_colour            'clear light colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.193
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3120
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.1
_refine_diff_density_max         0.347
_refine_diff_density_min         -0.225
_refine_diff_density_rms         0.050
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.076
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1032
_refine_ls_number_reflns         12830
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.076
_refine_ls_R_factor_all          0.0637
_refine_ls_R_factor_gt           0.0577
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0795P)^2^+3.8133P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1604
_refine_ls_wR_factor_ref         0.1659
_reflns_number_gt                11361
_reflns_number_total             12830
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3cp50757b.txt
_cod_data_source_block           mono_sad_100k
_cod_database_code               7211295